Page:NIOSH Manual of Analytical Methods - 9002.pdf/5

 ASBESTOS (bulk): METHOD 9002, Issue 2, dated 15 August 1994 - Page 5 of 9

j.

three, fibers will be straight, single fibers possibly with some larger composite fibers. Cleavage fragments may also be present. Examine using the central stop dispersion staining objective. Anthophyllite will exhibit central stop colors of blue and gold/gold-magenta; tremolite will exhibit pale blue and yellow; and actinolite will exhibit magenta and golden-yellow colors. NOTE: In this refractive index range, wollastonite is a common interfering mineral with similar morphology including the presence of cleavage fragments. It has both positive and negative sign of elongation, parallel extinction, and central stop dispersion staining colors of pale yellow and pale yellow to magenta. If further confirmation of wollastonite versus anthophyllite is needed, go to step "j". If any of the above forms of asbestos were confirmed above, go to step 15 for quantitative estimation. If none of the tests above confirmed asbestos fibers, examine the additional preparations and if the same result occurs, report the absence of asbestos in this sample. Wash a small portion of the sample in a drop of concentrated hydrochloric acid on a slide. Place the slide, with cover slip in place, on a warm hot plate until dry. By capillary action, place 1.620 RI liquid under the cover clip and examine the slide. Wollastonite fibers will have a "cross-hatched" appearance across the length of the fibers and will not show central stop dispersion colors. Anthophyllite and tremolite will still show their original dispersion colors. NOTE: There are alternative analysis procedures to the step-wise approach outlined above which will yield equivalent results. Some of these alternatives are: i. Perform the initial scan for the presence of asbestos using crossed polars as well as the first-order red compensator. This allows for simultaneous viewing of birefringent and amorphous materials as well as determine their sign of elongation. Some fibers which are covered with mortar may best be observed using this configuration. ii. Some analysts prefer to mount their first preparation in a RI liquid different than any asbestos materials and conduct their initial examination under plane-polarized light. iii. If alternative RI liquids are used from those specified, dispersion staining colors observed will also change. Refer to an appropriate reference for the specific colors associated with asbestos in the RI liquids actually used.

QUANTITATIVE ASSESSMENT: 15. Estimate the content of the asbestos type present in the sample using the 1.550 RI preparation. Express the estimate as an area percent of all material present, taking into account the loading and distribution of all sample material on the slide. Use Figure 1 as an aid in arriving at your estimate. If additional unidentified fibers are present in the sample, continue with the qualitative measurement (step 14). NOTE: Point-counting techniques to determine percentages of the asbestos minerals are not generally recommended. The point-counting method only produces accurate quantitative data when the material on the slide is homogeneous and has a uniform thickness, which is difficult to obtain [6]. The point-counting technique is, recommended by the EPA to determine the amount of asbestos in bulk [1]; however, in the more recent Asbestos Hazard Emergency Response Act (AHERA) regulations, asbestos quantification may be performed by a point-counting or equivalent estimation method [7]. 16. Make a quantitative estimate of the asbestos content of the sample from the appropriate combination of the estimates from both the gross and microscopic examinations. If asbestos fibers are identified, report the material as "asbestos-containing". Asbestos content should be reported as a range of percent content. The range reported should be indicative of the analyst's precision in estimating asbestos content. For greater quantities use Figure 1 in arriving at your estimate.

EVALUATION OF METHOD: The method is compiled from standard techniques used in mineralogy [8-13], and from standard laboratory procedures for bulk asbestos analysis which have been utilized for several years. These NIOSH Manual of Analytical Methods (NMAM), Fourth Edition, 8/15/94